#------------------------------------------------------------------------------
#$Date: 2025-03-04 20:56:51 +0200 (Tue, 04 Mar 2025) $
#$Revision: 298089 $
#$URL: file:///home/coder/svn-repositories/cod/cif/1/57/35/1573586.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1573586
loop_
_publ_author_name
'Kim, Hyunyong'
'Cohen, Seth M.'
_publ_section_title
;
 Metal-organic frameworks generated from oligomeric ligands with
 functionalized tethers.
;
_journal_issue                   5
_journal_name_full               'Chemical science'
_journal_page_first              2344
_journal_page_last               2350
_journal_paper_doi               10.1039/d4sc06666a
_journal_volume                  16
_journal_year                    2025
_chemical_formula_sum            'C96 O64 Zn16'
_chemical_formula_weight         3222.88
_space_group_crystal_system      cubic
_space_group_IT_number           225
_space_group_name_Hall           '-F 4 2 3'
_space_group_name_H-M_alt        'F m -3 m'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-2018/3
_audit_update_record
;
2024-11-27 deposited with the CCDC.	2025-01-07 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   25.6171(9)
_cell_length_b                   25.6171(9)
_cell_length_c                   25.6171(9)
_cell_measurement_reflns_used    5731
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      24.064
_cell_measurement_theta_min      2.637
_cell_volume                     16810.9(10)
_computing_cell_refinement       'APEX5 v2023.9-2 (Bruker, 2023)'
_computing_data_collection       'APEX5 v2023.9-2 (Bruker, 2023)'
_computing_data_reduction        'SAINT v8.40B (Bruker, 2019)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-2018/3 (Sheldrick, 2018)'
_computing_structure_solution    'SHELXT 2018/2 (Sheldrick, 2018)'
_diffrn_ambient_temperature      100(2)
_diffrn_measured_fraction_theta_full 0.994
_diffrn_measured_fraction_theta_max 0.995
_diffrn_measurement_device_type  'Bruker D8 Venture'
_diffrn_measurement_method       'ω and φ scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0571
_diffrn_reflns_av_unetI/netI     0.0160
_diffrn_reflns_Laue_measured_fraction_full 0.994
_diffrn_reflns_Laue_measured_fraction_max 0.995
_diffrn_reflns_limit_h_max       28
_diffrn_reflns_limit_h_min       -32
_diffrn_reflns_limit_k_max       32
_diffrn_reflns_limit_k_min       -32
_diffrn_reflns_limit_l_max       32
_diffrn_reflns_limit_l_min       -32
_diffrn_reflns_number            26386
_diffrn_reflns_point_group_measured_fraction_full 0.994
_diffrn_reflns_point_group_measured_fraction_max 0.995
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         26.945
_diffrn_reflns_theta_min         2.637
_diffrn_source                   'Micro Focus Rotating Anode'
_exptl_absorpt_coefficient_mu    1.153
_exptl_absorpt_correction_T_max  0.893
_exptl_absorpt_correction_T_min  0.767
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   SADABS-2016/2
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    0.637
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       cubic
_exptl_crystal_F_000             3136
_exptl_crystal_size_max          0.200
_exptl_crystal_size_mid          0.100
_exptl_crystal_size_min          0.100
_refine_diff_density_max         0.473
_refine_diff_density_min         -0.247
_refine_diff_density_rms         0.061
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.125
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     31
_refine_ls_number_reflns         973
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.125
_refine_ls_R_factor_all          0.0835
_refine_ls_R_factor_gt           0.0589
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.1281P)²+24.0299P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1925
_refine_ls_wR_factor_ref         0.2234
_reflns_Friedel_coverage         0.000
_reflns_number_gt                651
_reflns_number_total             973
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            d4sc06666a2.cif
_cod_data_source_block           oligoIRMOF-1-L6
_cod_depositor_comments
'Adding full bibliography for 1573584--1573593.cif.'
_cod_original_cell_volume        16810.9(18)
_cod_database_code               1573586
_shelx_shelxl_version_number     2018/3
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_min   0.802
_shelx_estimated_absorpt_t_max   0.893
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, z'
'-x, y, -z'
'x, -y, -z'
'z, x, y'
'z, -x, -y'
'-z, -x, y'
'-z, x, -y'
'y, z, x'
'-y, z, -x'
'y, -z, -x'
'-y, -z, x'
'y, x, -z'
'-y, -x, -z'
'y, -x, z'
'-y, x, z'
'x, z, -y'
'-x, z, y'
'-x, -z, -y'
'x, -z, y'
'z, y, -x'
'z, -y, x'
'-z, y, x'
'-z, -y, -x'
'x, y+1/2, z+1/2'
'-x, -y+1/2, z+1/2'
'-x, y+1/2, -z+1/2'
'x, -y+1/2, -z+1/2'
'z, x+1/2, y+1/2'
'z, -x+1/2, -y+1/2'
'-z, -x+1/2, y+1/2'
'-z, x+1/2, -y+1/2'
'y, z+1/2, x+1/2'
'-y, z+1/2, -x+1/2'
'y, -z+1/2, -x+1/2'
'-y, -z+1/2, x+1/2'
'y, x+1/2, -z+1/2'
'-y, -x+1/2, -z+1/2'
'y, -x+1/2, z+1/2'
'-y, x+1/2, z+1/2'
'x, z+1/2, -y+1/2'
'-x, z+1/2, y+1/2'
'-x, -z+1/2, -y+1/2'
'x, -z+1/2, y+1/2'
'z, y+1/2, -x+1/2'
'z, -y+1/2, x+1/2'
'-z, y+1/2, x+1/2'
'-z, -y+1/2, -x+1/2'
'x+1/2, y, z+1/2'
'-x+1/2, -y, z+1/2'
'-x+1/2, y, -z+1/2'
'x+1/2, -y, -z+1/2'
'z+1/2, x, y+1/2'
'z+1/2, -x, -y+1/2'
'-z+1/2, -x, y+1/2'
'-z+1/2, x, -y+1/2'
'y+1/2, z, x+1/2'
'-y+1/2, z, -x+1/2'
'y+1/2, -z, -x+1/2'
'-y+1/2, -z, x+1/2'
'y+1/2, x, -z+1/2'
'-y+1/2, -x, -z+1/2'
'y+1/2, -x, z+1/2'
'-y+1/2, x, z+1/2'
'x+1/2, z, -y+1/2'
'-x+1/2, z, y+1/2'
'-x+1/2, -z, -y+1/2'
'x+1/2, -z, y+1/2'
'z+1/2, y, -x+1/2'
'z+1/2, -y, x+1/2'
'-z+1/2, y, x+1/2'
'-z+1/2, -y, -x+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, -y+1/2, z'
'-x+1/2, y+1/2, -z'
'x+1/2, -y+1/2, -z'
'z+1/2, x+1/2, y'
'z+1/2, -x+1/2, -y'
'-z+1/2, -x+1/2, y'
'-z+1/2, x+1/2, -y'
'y+1/2, z+1/2, x'
'-y+1/2, z+1/2, -x'
'y+1/2, -z+1/2, -x'
'-y+1/2, -z+1/2, x'
'y+1/2, x+1/2, -z'
'-y+1/2, -x+1/2, -z'
'y+1/2, -x+1/2, z'
'-y+1/2, x+1/2, z'
'x+1/2, z+1/2, -y'
'-x+1/2, z+1/2, y'
'-x+1/2, -z+1/2, -y'
'x+1/2, -z+1/2, y'
'z+1/2, y+1/2, -x'
'z+1/2, -y+1/2, x'
'-z+1/2, y+1/2, x'
'-z+1/2, -y+1/2, -x'
'-x, -y, -z'
'x, y, -z'
'x, -y, z'
'-x, y, z'
'-z, -x, -y'
'-z, x, y'
'z, x, -y'
'z, -x, y'
'-y, -z, -x'
'y, -z, x'
'-y, z, x'
'y, z, -x'
'-y, -x, z'
'y, x, z'
'-y, x, -z'
'y, -x, -z'
'-x, -z, y'
'x, -z, -y'
'x, z, y'
'-x, z, -y'
'-z, -y, x'
'-z, y, -x'
'z, -y, -x'
'z, y, x'
'-x, -y+1/2, -z+1/2'
'x, y+1/2, -z+1/2'
'x, -y+1/2, z+1/2'
'-x, y+1/2, z+1/2'
'-z, -x+1/2, -y+1/2'
'-z, x+1/2, y+1/2'
'z, x+1/2, -y+1/2'
'z, -x+1/2, y+1/2'
'-y, -z+1/2, -x+1/2'
'y, -z+1/2, x+1/2'
'-y, z+1/2, x+1/2'
'y, z+1/2, -x+1/2'
'-y, -x+1/2, z+1/2'
'y, x+1/2, z+1/2'
'-y, x+1/2, -z+1/2'
'y, -x+1/2, -z+1/2'
'-x, -z+1/2, y+1/2'
'x, -z+1/2, -y+1/2'
'x, z+1/2, y+1/2'
'-x, z+1/2, -y+1/2'
'-z, -y+1/2, x+1/2'
'-z, y+1/2, -x+1/2'
'z, -y+1/2, -x+1/2'
'z, y+1/2, x+1/2'
'-x+1/2, -y, -z+1/2'
'x+1/2, y, -z+1/2'
'x+1/2, -y, z+1/2'
'-x+1/2, y, z+1/2'
'-z+1/2, -x, -y+1/2'
'-z+1/2, x, y+1/2'
'z+1/2, x, -y+1/2'
'z+1/2, -x, y+1/2'
'-y+1/2, -z, -x+1/2'
'y+1/2, -z, x+1/2'
'-y+1/2, z, x+1/2'
'y+1/2, z, -x+1/2'
'-y+1/2, -x, z+1/2'
'y+1/2, x, z+1/2'
'-y+1/2, x, -z+1/2'
'y+1/2, -x, -z+1/2'
'-x+1/2, -z, y+1/2'
'x+1/2, -z, -y+1/2'
'x+1/2, z, y+1/2'
'-x+1/2, z, -y+1/2'
'-z+1/2, -y, x+1/2'
'-z+1/2, y, -x+1/2'
'z+1/2, -y, -x+1/2'
'z+1/2, y, x+1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, y+1/2, -z'
'x+1/2, -y+1/2, z'
'-x+1/2, y+1/2, z'
'-z+1/2, -x+1/2, -y'
'-z+1/2, x+1/2, y'
'z+1/2, x+1/2, -y'
'z+1/2, -x+1/2, y'
'-y+1/2, -z+1/2, -x'
'y+1/2, -z+1/2, x'
'-y+1/2, z+1/2, x'
'y+1/2, z+1/2, -x'
'-y+1/2, -x+1/2, z'
'y+1/2, x+1/2, z'
'-y+1/2, x+1/2, -z'
'y+1/2, -x+1/2, -z'
'-x+1/2, -z+1/2, y'
'x+1/2, -z+1/2, -y'
'x+1/2, z+1/2, y'
'-x+1/2, z+1/2, -y'
'-z+1/2, -y+1/2, x'
'-z+1/2, y+1/2, -x'
'z+1/2, -y+1/2, -x'
'z+1/2, y+1/2, x'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Zn1 Zn 0.70645(2) 0.29355(2) 0.70645(2) 0.0675(5) Uani 1 6 d S T P . .
O1 O 0.750000 0.250000 0.750000 0.059(2) Uani 1 24 d S T P . .
O2 O 0.71868(17) 0.36634(19) 0.71868(17) 0.144(2) Uani 1 2 d S T P . .
C1 C 0.750000 0.4463(3) 0.750000 0.126(4) Uani 1 4 d S T P . .
C2 C 0.750000 0.3886(3) 0.750000 0.120(3) Uani 1 4 d S T P . .
C3 C 0.7830(3) 0.4732(3) 0.7830(3) 0.151(4) Uani 1 2 d S T P . .
O3 O 0.8163(8) 0.4520(8) 0.8163(8) 0.208(15) Uani 0.25 2 d S T P . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Zn Zn 0.2839 1.4301 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O2 Zn1 O2 106.9(2) . 12_665 ?
O2 Zn1 O2 106.9(2) . 6_566 ?
O2 Zn1 O2 106.9(2) 12_665 6_566 ?
O2 Zn1 O1 111.90(18) . . ?
O2 Zn1 O1 111.90(18) 12_665 . ?
O2 Zn1 O1 111.90(18) 6_566 . ?
O2 Zn1 Zn1 76.63(18) . 51_656 ?
O2 Zn1 Zn1 124.92(14) 12_665 51_656 ?
O2 Zn1 Zn1 124.92(14) 6_566 51_656 ?
O1 Zn1 Zn1 35.264(1) . 51_656 ?
O2 Zn1 Zn1 124.91(14) . 28_556 ?
O2 Zn1 Zn1 76.63(18) 12_665 28_556 ?
O2 Zn1 Zn1 124.92(14) 6_566 28_556 ?
O1 Zn1 Zn1 35.264(1) . 28_556 ?
Zn1 Zn1 Zn1 60.0 51_656 28_556 ?
O2 Zn1 Zn1 124.91(14) . 74_655 ?
O2 Zn1 Zn1 124.92(14) 12_665 74_655 ?
O2 Zn1 Zn1 76.63(18) 6_566 74_655 ?
O1 Zn1 Zn1 35.264(1) . 74_655 ?
Zn1 Zn1 Zn1 60.000(1) 51_656 74_655 ?
Zn1 Zn1 Zn1 60.0 28_556 74_655 ?
Zn1 O1 Zn1 109.471(1) 51_656 28_556 ?
Zn1 O1 Zn1 109.471(2) 51_656 74_655 ?
Zn1 O1 Zn1 109.471(1) 28_556 74_655 ?
Zn1 O1 Zn1 109.5 51_656 . ?
Zn1 O1 Zn1 109.471(1) 28_556 . ?
Zn1 O1 Zn1 109.471(2) 74_655 . ?
C2 O2 Zn1 130.0(5) . . ?
C3 C1 C3 120.0(9) . 51_656 ?
C3 C1 C2 120.0(5) . . ?
C3 C1 C2 120.0(5) 51_656 . ?
O2 C2 O2 126.7(9) . 51_656 ?
O2 C2 C1 116.7(4) . . ?
O2 C2 C1 116.7(4) 51_656 . ?
O3 C3 C3 114.2(11) . 99_565 ?
O3 C3 C1 125.8(12) . . ?
C3 C3 C1 120.0(5) 99_565 . ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Zn1 O2 1.917(5) . ?
Zn1 O2 1.917(5) 12_665 ?
Zn1 O2 1.917(5) 6_566 ?
Zn1 O1 1.9323(10) . ?
Zn1 Zn1 3.1554(16) 51_656 ?
Zn1 Zn1 3.1554(16) 28_556 ?
Zn1 Zn1 3.1554(16) 74_655 ?
O2 C2 1.270(6) . ?
C1 C3 1.379(10) . ?
C1 C3 1.379(10) 51_656 ?
C1 C2 1.479(12) . ?
C3 O3 1.33(3) . ?
C3 C3 1.371(15) 99_565 ?
